Ultrasonics xxx (xxxx) xxx–xxx
Contents lists available at ScienceDirect
Ultrasonics journal homepage: www.elsevier.com/locate/ultras
One-step polymeric phononic crystal manufacture ⁎
Nan Lia, , Christopher R. Loweb, Adrian C. Stevensona a b
Department of Chemical Engineering and Biotechnology, University of Cambridge, Philippa Fawcett Drive, Cambridge, CB3 0AS, UK Cambridge Academy of Therapeutic Sciences, University of Cambridge, 17 Mill Lane, Cambridge, CB2 1RX, UK
A R T I C LE I N FO
A B S T R A C T
Keywords: Phononic crystal Metamaterial Slow wave eﬀect Bulk acoustic waves Standing wave Polyacrylamide
A versatile system to construct bulk polymeric phononic crystals by using acoustic waves is described. In order to fabricate this material, a customised cavity device ﬁtted with a 2 MHz acoustic transducer and an acoustic reﬂector is employed for the acoustic standing wave creation in the device chamber. The polymer crystal is formed when the standing waves are created during the polymerisation process. The resulting crystals are reproduced into the shape of the tunable device cavity with a unique periodic feature. The separation is related to the applied acoustic wave frequency during the fabrication process and each unit cell composition was found to be made up to two material phases. To assess the acoustic properties of the polymer crystals their average acoustic velocity is measured relative to monomer solutions of diﬀerent concentrations. It is demonstrated that one of the signature characteristics of phononic crystal, the slow wave eﬀect, was expressed by this polymer. Furthermore the thickness of a unit cell is analysed from images obtained with microscope. By knowing the thickness the average acoustic velocity is calculated to be 1538 m/s when the monomer/cross-linker concentration is 1.5 M. This numerical calculation closely agrees with the predicted value for this monomer/crosslinker concentration of 1536 m/s. This work provides a methodology for rapid accessing a new type of adaptable phononic crystal based on ﬂexible polymers.
1. Introduction Phononic crystals occur naturally as the result of the periodic nature of atomic crystals. The concept of artiﬁcial phononic crystals was proposed decades ago [1,2] and signiﬁcant interest has followed since, but not limited to one form [3–9]. The attraction is that these materials can potentially address enduring engineering challenges in acoustics as they introduce physical eﬀects that change the very nature of acoustic wave excitation and propagation. They can be commonly achieved by periodically altering the density or bulk modulus, so that the acoustic waves propagation depends on wavelength, which in turn alters the non-linear properties of the material. Alternatively for subwavelength periodicity evanescent acoustic surface waves have also been employed . Together the breadth of phononic crystal applications is considerable. With band gap and band edge states phononic crystals are able to disperse the group velocity and bend acoustic waves [11,12], leading to applications including signal processing [13,14] and opportunities to reduce thermal conductivity [15,16]. This rapidly growing ﬁeld of study originated in bulk materials, however it was diﬃcult to produce the periodic properties. Initially this was achieved by combining bulk acoustic wave devices to make ﬁlters. This activity became easier with surface acoustic wave devices and ⁎
their metallic grating [10,17]. These have provided excellent acoustic propagation control, and so these devices control acoustic waves to provide signal processing for mobile phones. A key development is the interdigitated electrode structure. A periodic metal pattern is formed on a substrate, and interacts with a surface acoustic wave (SAW), typically a Rayleigh wave. Taking SAW devices as the platform, surface phononic crystals are able to exercise interrogation on thin soft polymer in conjunction with opto-acoustic transducers [18,19] and increase transmitting pulse temporal beating . Unfortunately this method cannot be used for bulk materials, so it cannot be used to modulate sound transmission in the larger environment. Nevertheless some attempts have been made to create bulk phononic crystals as a ﬁrst step to creating acoustic metamaterials. As a newly emerging ﬁeld metamaterials display counter-intuitive physical eﬀects. Due to the Bragg scattering caused by impedance contrast of the mass density or the elastic moduli, useful acoustic dispersion, band gap and slow wave effect emerge. Although the theoretical research of phononic crystals is rich in numerical models, fabrications methods are rare. These broadly consist of solid sphere arrays embedded in soft matrix [21–24]. Or more recently, 3D printing technology is used for phononic crystal fabrication  and interference lithographic template assisted three-dimensional elastomeric network production [26,27]. Because of these limited
Corresponding author. E-mail address: [email protected]
https://doi.org/10.1016/j.ultras.2018.07.001 Received 31 January 2018; Received in revised form 5 July 2018; Accepted 6 July 2018 0041-624X/ © 2018 Elsevier B.V. All rights reserved.
Please cite this article as: Li, N., Ultrasonics (2018), https://doi.org/10.1016/j.ultras.2018.07.001
Ultrasonics xxx (xxxx) xxx–xxx
N. Li et al.
subsequent interaction of developed polymer crystals with acoustic waves, a series of average acoustic velocity measurements have been obtained at room temperature. The following subsections present the design concept of this adjustable cavity device, the procedure for fabricating the polymeric phononic crystal and the acoustic velocity measurements needed to characterise the material.
options, most of these crystals are slowly built layer by layer or extensively delicate processes are necessitated. We report a versatile method to add multiple periodic features using a monomer/cross-linker solution as a starting point. This method applies megahertz acoustic standing waves to an acrylamide system undergoing a polymerisation process and consequentially a bulk polymeric phononic crystal is fabricated. In the following sections we consider the theory of phononic crystals alongside bulk grating approaches. The standing wave imprinting device, formulation of monomer/cross-linker mix are described. The polymer images, imprinting mechanism and acoustic transmission properties associated with these polymeric phononic crystals are analysed and discussed.
3.1. Adjustable polymeric phononic crystal fabrication tube The basic design concept allows ﬂexible creation of polymer crystals. It functions by projecting wave energy into the device cavity chamber which in turn contain trapped standing waves. Here the pressure waves interact with the liquid phase monomer/cross-linker. The resulting acoustic ﬁeld depends on constructive and destructive interference of the acoustic waves which depend on sample properties and separation of the transducer and reﬂector. The distance is tuned to be a multiple of half wavelength to form the standing wave. Hence this design allows path length phase adjustment between the transducer and the reﬂector, which is essential for fabricating high quality polymer crystals. The main device body consists of a glass tube (Soham Scientiﬁc, Ely, UK) with an inner diameter of 30 mm. The space available for the monomer solution is conﬁned within the glass tube by two circular discs made from polytetraﬂuoroethylene (PTFE). One incorporates a 2 MHz acoustic transducer of 25 mm in diameter (Noliac, Denmark) whilst the other supports an acoustic reﬂector made from stainless steel. The distance between the transducer and the steel reﬂector can be regulated by a translation screw that converts rotary motion into the linear disc motion inside the glass tube (Fig. 1). To maximise the reﬂected acoustic waves so that energy is largely trapped in the tube, the acoustic reﬂector is selected to maximise the acoustic impedance mismatch between medium and reﬂector. The acoustic impedance of the monomer solution is assumed to equal water at 1.48 MRayl at 20 °C . The properties of potential materials are listed in Table 1. They are sorted in descending order according to their reﬂection coeﬃcient R. Platinum or gold produces the best reﬂection performance, however for this application the stainless steel disc is more accessible and practical.
2. Theory The applications of acoustics often involve the interaction of waves at the acoustic boundaries. Acoustic reﬂection occurs along a path associated with the incident wave. Only part of the incident wave energy transmits from the ﬁrst medium, referred as medium m here, into the second medium, referred as reﬂector r here. The most basic acoustic properties that determine this include the medium elasticity and density. The elasticity and density of a medium determine the acoustic impedance Z, which in turn governs the transmission coeﬃcient T and the reﬂection coeﬃcient R. Both T and R are independent from the energy ﬂow direction. Under the condition of normal incidence,
R = 1−T =
Zr −Zm Zr + Zm
A typical acoustic phononic crystal is a collective cluster of a number of unit cells made up of two layers with an acoustic boundary in between. To comprehend the waves propagation in a periodic structure, it is essential to understand the nature of the wave eigenmode in it. Bloch indicated that a wave propagating in a periodic structure is a superposition of a series of plane wave . The Bloch theorem is expressed as:
ψk (r ) = uk (r ) eikr
where k is the wave vector, r is the position, e is Euler’s number, i is the imaginary unit. uk (r ) is the periodic function of the crystal lattice with uk (r ) = uk (r + R) in which R is the periodicity of the crystal lattice. Being diﬀerent from the velocity deﬁnition of a particle, waves have three types of velocities, including phase velocity vph , group velocity vg and energy velocity ve , amongst which vph refers to the propagation of an equiphase surface; the group velocity to the propagation of a wave pocket; and the energy velocity to the propagation of energy. The group velocity is proved to be equivalent to the energy velocity of a Bloch wave , i.e.:
s ∂ω (k r ) = k = ve wk ∂k r
3.2. Polymeric phononic crystal fabrication The periodic structure that emerges is associated with the acoustic standing wave ﬁeld in the fabrication tube chamber. An HP 33120A signal generator in-line with an ENI 310L power ampliﬁer is arranged to excite the piezo disc. Fig. 2 illustrates the fabrication setup. A 4 mL monomer/cross-linker solution containing 98.5 mol% acrylamide and 1.5 mol% N,N′-methylenebisacrylamide (MBA) is used to ﬁll the fabrication tube. The chemical initiators, including 48 μL 10%(w/v) freshly prepared ammonium persulfate (APS) and 4 μL tetramethylethylenediamine (TEMED) are loaded and the chemical inlet sealed. The tube is shaken gently to achieve thorough mixing of the reagents. The device is left on the table in a secure horizontal position.
where ωr (k ) holds dispersion relation with k r , sk = 〈s〉|ω (kr ) and wk = 〈w〉|ω (kr ) are the average wave energy ﬂow density and wave energy density respectively. While the phase velocity applies to a wave at single frequency, i.e.vph = ω/ k . A key feature is when the length scale of the periodic structure is comparable to the wavelength of the wave, the excitation of the unit cells leads to a strong resonant scattering. Thus the action of the phononic crystal can be evidenced by this strong resonant scattering and a ”slow wave eﬀect” [11,12].
Fig. 1. Phononic crystal fabrication tube. The acoustic waves arise from the acoustic transducer and reﬂect at the boundary between the medium and the acoustic reﬂector. The incident wave interacts with the reﬂected wave constructing an acoustic standing wave. The distance between the acoustic transducer and reﬂector can be adjusted by turning the translation screw attached to the left PTFE disc. The chemicals are fed into the glass tube through the chemical inlet on top of the tube.
3. Experimental setup In order to fabricate the polymer crystal, a bespoke ultrasonic cavity chamber is employed for holding the monomer/cross-linker solution within the ﬁeld of deﬁned acoustic standing waves. To assess the 2
Ultrasonics xxx (xxxx) xxx–xxx
N. Li et al.
Table 1 Acoustic properties of selected solid materials  This table is sorted according to the reﬂection coeﬃcient R in descending order. vl is the longitudinal acoustic wave travelling speed; ρ is the density; Z is the acoustic impedance. Material
Platinum Gold Stainless steel Copper Silver Brass Titanium Iron cast Lead Aluminium Glass silica Polystyrene
3.26 3.24 5.79 5.01 3.60 4.70 8.27 5.90 2.20 6.42 5.90 2.34
21.40 19.70 7.69 8.93 1.60 8.64 5.15 7.69 11.20 2.70 2.20 1.04
84.74 62.60 45.63 41.46 37.76 37.30 27.69 25.00 24.49 17.33 13.00 2.47
0.966 0.954 0.937 0.931 0.925 0.924 0.899 0.888 0.886 0.840 0.796 0.251
Table 2 Coeﬃcients for acoustic velocity calculation in water. i
0 1 2
1404.30 4.70 −0.04
generated by the transducer A travels through the tank media to reach transducer B. If a polymer block is placed in path A-B a time diﬀerence Δt results. Rearranging the time diﬀerence calculation Eq. (4), Eq. (5) gives the average acoustic velocity through the polymer alone, cp .
thp Δt + thp/ c w
where thp is the polymer thickness measured with a digital calliper. To minimise measurement error due to the polymer creep, hard plastic discs of known thickness are placed on either side of the polymer crystal during measurement. c w is the acoustic velocity in water and depends on temperature. c w used in this study is calculated from a quadratic 2 equation c w = ∑i = 0 ki T i . This simpliﬁed equation is reasonably accurate over the 15–35 °C temperature range . The coeﬃcient ki are given in Table 2 and T is the temperature of water in Celsius. The water temperature used for the velocity measurements is controlled at 23 ± 0.2 °C and corresponds to 1491 m/s.
Fig. 2. The polymeric phononic crystal fabrication setup. The acoustic transducer in the fabrication tube is actuated by a signal generator, which passes through a power ampliﬁer before the electric signal reaches the transducer.
4. Results and discussion
The signal generator energises the piezo disc (Noliac Ceramics NCE51) at Vpp 90 mV at its resonant frequency. The translation screw knob is adjusted and a periodic structure forms in the tube that is clearly visible to the naked eye. The distance between the piezo disc and the stainless steel reﬂector is approximately ∼6 mm. The polymerisation process takes less than 1 min. The signal generator and the ampliﬁer are switched oﬀ at a predetermined time corresponding to the onset of polymer rigidiﬁcation.
4.1. The polymeric crystal The nature of the polymer crystal is related to the acoustic standing wave ﬁeld and the shape of the fabrication tube. The process employed for making the polymer crystal is described in Section 3.2. The resulting crystal after stabilisation is a 6 mm thick polymer disc with a diameter of 30 mm. Importantly, the disc contains distinct layers that can be seen by the naked eye. To help interpret the nature of layers we consider a simpliﬁed approach here. The mechanism determining the formation of the polymer crystal is still unconﬁrmed. Nevertheless the resulting patterns deﬁnitely emerge from pressure wave action on the monomer mix during the crosslinking process. If we move forward with a simple interpretative models, it is reasonable to conclude the rate of polymer cross linking is proportional to the amplitude of the acoustic standing wave. Thus subject to the nodal or antinodal conditions the resulting material is likely to be biphasic, i.e. containing two diﬀerent mechanical phases. Here the antinodes should produce a stiﬀer material and conversely at the nodes a less stiﬀ material. Thus light passing through the polymer may experience a diﬀerence in propagation path leading to a visible contrast, which matches our experimental observations. Optical microscopy was used to evaluate the quality of the crystals formed. A 1 mm thick piece of polymer crystal was used to assess line deﬁnition and spacing. This was sliced perpendicular to the radial plane with the cross-section facing the lens of a 4× magniﬁcation microscope. The grey values of the selected cross-section area is plotted as a 3D surface shown in Fig. 5(a). To assist with periodicity analysis, a proﬁle analysis was performed and shown in Fig. 5(b). The pixel grey values along a line are presented in Fig. 5(c) z-axis. Two light and shaded striations stand out signifying a biphasic material form. Based on an average wavelength of 0.712 ± 0.0077 mm (8 measurements) and a 2.16 MHz standing wave frequency the average acoustic velocity was found to be 1538 m/s, which is consistent with interpolated values for
3.3. Acoustic velocity measurement of the polymer To investigate any slowing eﬀect on acoustic waves we measured their average acoustic velocities and compared to their counterparts using a pulsed based setup. Fig. 3 illustrates how the acoustic velocity through a polymer block is measured. An acoustic signal burst
Fig. 3. Experimental method to determine the average acoustic velocity across the polymer. The acoustic bursts travelling time diﬀerence Δt = t1−t2 is recorded, where t1 is the time that an acoustic burst travels from acoustic transducer A to B without a polymer block in between, while t2 is the travelling time when a polymer is placed between A and B. 3
Ultrasonics xxx (xxxx) xxx–xxx
N. Li et al.
Fig. 4. Phononic structures made with 4 MHz (b) PC_I and 2 MHz (b) PC_II acoustic transducers. The labels h1 and h2 (a) are of the same length. While h1 covers about two spacial periodicities of the phononic crystal shown on PC_I, h2 covers only one of PC_II.
acoustic velocity vs. acrylamide concentration in Section 4.3. Here the patterns were coherent and consistently well-formed. The transducer frequency determines the spacing in the crystal structure. The data shown in Fig. 4 reveals the patterns can be formed with the periodicity decreasing proportionally with frequency. This is evidenced by the factor 2 increase in frequency yielding the expected factor 2 reduction in periodicity. Thus the microscopy data reveals contrast that is linked to material changes, so alternating bright and dark regions are a record of the acoustic ﬁeld during crosslinking. However it is unproven whether the ﬂuctuations in brightness are due to a mechanical periodicity. Fig. 6. The SEM images taken of the polymer at two diﬀerent magniﬁcations conﬁrm that the acoustic standing wave records periodic mechanical variations in the monomer mix.
4.2. The structured polymer under scanning electron microscope (SEM) SEM data was used to conﬁrm mechanical periodicity in the polymer crystal. Here the SEM data in Fig. 6 shows the cross-section
topology is periodic indicating an underlying variation of hills and valleys across the sample cross-section. Furthermore these regions include elongated voids and circular voids, conﬁrming the recording of entrenched periodic mechanical properties by the standing wave. Thus it would imply the inherent potential to scatter an acoustic wave. Freeze drying of the acrylamide polymers was found to reduce structural coherence by imposing unequal forces on the structure. Thus the SEM images which were useful in identifying the mechanical periodicity of polymer, also conﬁrms that drying of the polymer will distort the structure. Thus water content does inﬂuence the coherence of these polymer crystals. As crystallisation patterns have been successfully recorded and conﬁrmed the optical and SEM data it is useful to study acoustic wave transmission through them. In particular based on the theory of “the slow wave eﬀect” we investigate the important scattering and velocity relationship. 4.3. Average acoustic velocity across the polymer We investigated the relation between the acoustic velocities of polymer crystals according to diﬀerent polyacrylamide concentrations. As a reference point the signal from the counterpart material was also measured. These counterparts are fabricated in the same cavity device and corresponding acrylamide solutions, but during polymerisation the acoustic standing wave ﬁeld is absent. Therefore no periodic structure emerges. The polymer explore acrylamide concentrations between 5%(w/v) and 40%(w/v) in 5%(w/v) intervals. The corresponding polymer acoustic velocities are presented in Fig. 7. A positive linear correlation between the acrylamide concentration and average acoustic velocity is observed. The general linear model function in SPSS reveals a correlation between the concentration of acrylamide and acoustic velocity across the polymer crystal. The pvalue of interest is 0.001. The fact that it is smaller than the
Fig. 5. Optical images of a high quality polymer crystal: (a) is a simulated 3D proﬁle via the 3D spectrum plot. Here the z-axis shows the grey value where 0 represents black and 255 is white, and the x-axis is perpendicular to the direction of the periodic structure and y-axis is parallel. (b) Shows the original selected region that formed the presented in (c). 4
Ultrasonics xxx (xxxx) xxx–xxx
N. Li et al.
Fig. 7. Acoustic velocities across the polyacrylamide based phononic crystals and their counterparts made from a series of concentration monomer solutions.
predetermined signiﬁcance level 0.05 suggests these two ﬁtting lines are independent. A key ﬁnding is the average acoustic velocity (at 1 MHz) of the polymer crystals is lower than their bulk polymer counterparts. This agrees with the slow wave eﬀect. Here the periodic structure of a phononic crystal interacts with the waves. Although the temporal coherence is maintained with the incident acoustic wave, the scattering has a noticeable impact on the group velocity . In Section 4.1 the optical evaluation of a slice of the polymer crystal indicates the average acoustic velocity through it is 1538 m/s. The monomer/cross-linker solution used in that experiment is 1.5 M equivalent to 10.85%(w/v). Substitute the acrylamide factor with 10.85%(w/v) in the orange ﬁtting line in Fig. 7, it gives an average acoustic velocity 1536 m/s as a result in accordance with the optical evaluation value. One may argue that when the monomer concentration is 0%(w/v), the acoustic velocity cm should approach pure water c w , i.e. lim% (w / v) → 0 cm = c w . The intercepts for both ﬁtting lines thus should have been set at the acoustic velocity of water at ambient temperature. However, it must be noted for pure water, the acoustic standing wave still induces a periodic structure as shown in Fig. 8. Thus the surprising result is that a temporary periodic ﬁeld can also lead to a velocity shift. The partitioning mechanism leading to the formation of a unique periodic structure in polyacrylamide is complex. Copolymerisation of acrylamide and MBA is already more involved than the standard free radical polymerisation . One perspective is that when polymerisation is taking place, a sequence of events occurs in the micro-environment varying pressure and energy and physico-chemical conditions over time and space. This exacerbates polymerisation complexity. Thus a working hypothesis which is one of several yet to be conﬁrmed, is that the acoustic standing waves promote a density diﬀerential over space. As the polymer chains elongate, they become insoluble and precipitate. These precipitates have a diﬀerent density and compressibility from the solution. As the acoustic pressure gradient from standing wave prevails, the partially polymerised matter appearing at the antinodes moves towards the pressure nodes, as is demonstrated in Fig. 9(a), assuming the acoustic contrast factor is positive. Meanwhile, the monomer concentration and cross-linker also aﬀect the polymer elasticity modulus and density . Upon completion of the standing wave polymerisation, the polymer in the nodal regions is denser and more cross-linked than the antinodal regions (Fig. 9(b)). Overall more investigation of the event sequence is needed to isolate the mechanism.
Fig. 8. The periodicity introduced in pure water by acoustic standing waves. (a) Shows the periodic structure formed within the fabrication tube. (b) Is a selected zoom-in region on (a). λ w is the wavelength of acoustic wave in water and λ w /2 labels one unit of the periodicity. (c) Is the 2D Fourier Transform of (b) that conﬁrms the periodic phononic crystal state.
Fig. 9. The standing wave enabled polymeric phononic crystal formation hypothesis: (a) Partially polymerised precipitants emerge from stimulated radical activity at the peak pressure ﬁeld (antinodes) while being propelled to the pressure nodes at the early polymerisation stage. (b) Towards the end of the polymerisation, the polymer locating at the pressure nodes is denser due to mass accumulation and packing within the nodal proﬁle. Thus within the acoustic ﬁeld the structure adapts to minimise its energy.
cross-linking, comprises a monomer/cross-linker solution plus polymerisation chemical initiators. The resulting form of the polymer crystal follows the cylindrical shape of the fabrication tube producing 30 distinctive layers, which have alternating refractive indices that are visible to naked eye. The resultant polymeric phononic crystals were investigated by observing under an optical microscope and in transmission via an SEM. The latter provides detailed information on the periodic structure, the pore sizes in the polymer and the scale of the change. Visualising the periodic structure and determining its periodicity, provides an approximate calculation of the average acoustic velocity across the
5. Conclusion A novel approach for fabricating bulk polymeric phononic crystals with acoustic standing waves has been demonstrated. The cavity device follows a well established approach to create a standing wave ﬁeld suitable for the polymer transformation. The starting form, prior to 5
Ultrasonics xxx (xxxx) xxx–xxx
N. Li et al.
phononic crystal. The value 1538 m/s closely agrees with the interpolated value from the direct acoustic velocity measurements 1536 m/ s. The refractive index diﬀerences can be attributed to variable monomer concentration aﬀecting the elasticity. The acoustic velocity of pulses travelling through these phononic crystals and their counterparts are evaluated. The group velocity of the phononic crystals shows a lower acoustic velocity relative to counterparts of the same shape that omit periodic structures. These measurements match with theoretical studies of the behaviour of the slow wave eﬀect in phononic crystals. Contrasting with existing work this rapid fabrication approach does not necessitate the inclusion of particles, reducing complexity and saving fabrication time and costs. In its native form it is capable of creating unit cells from the standing wave planes adding important local resonance behaviour to the polymer. Thus it provides a signiﬁcant short-cut for fabricating bulk polymeric phononic crystals at both small and large scales within the period of minutes, and can be adapted to a manufacturing process. This technique may also be extended to fabricate phononic crystals at a wider frequency spectrum and beneﬁt larger range of metamaterial fabrication.
The authors are grateful to Dr. Jeremy Skepper for assistance with SEM imaging of the sample, to Dr. Ke Xu Zhou for helpful discussions on the mechanism and to Mr. Lee Pratt for the machining of the adjustable polymeric phononic crystal fabrication tube. For part of this work, Dr. Nan Li was funded by the Cambridge Overseas Trust.
   
 L. Brillouin, M. Parodi, Propagation of waves in periodic structures, Foreign Lit. (1953).  M.S. Kushwaha, P. Halevi, L. Dobrzynski, B. Djafari-Rouhani, Acoustic band structure of periodic elastic composites, Phys. Rev. Lett. 71 (1993) 2022.  S. Yang, J.H. Page, Z. Liu, M.L. Cowan, C.T. Chan, P. Sheng, Focusing of sound in a 3D phononic crystal, Phys. Rev. Lett. 93 (2004) 024301.  X. Zhang, Z. Liu, Negative refraction of acoustic waves in two-dimensional phononic crystals, Appl. Phys. Lett. 85 (2004) 341–343.  C. Qiu, Z. Liu, J. Shi, C. Chan, Directional acoustic source based on the resonant cavity of two-dimensional phononic crystals, Appl. Phys. Lett. 86 (2005) 224105.  C. Qiu, Z. Liu, Acoustic directional radiation and enhancement caused by band-edge states of two-dimensional phononic crystals, Appl. Phys. Lett. 89 (2006) 063106.  N. Fang, D. Xi, J. Xu, M. Ambati, W. Srituravanich, C. Sun, X. Zhang, Ultrasonic metamaterials with negative modulus, Nat. Mater. 5 (2006) 452–456.  L. Feng, X.-P. Liu, M.-H. Lu, Y.-B. Chen, Y.-F. Chen, Y.-W. Mao, J. Zi, Y.-Y. Zhu, S.N. Zhu, N.-B. Ming, Acoustic backward-wave negative refractions in the second band of a sonic crystal, Phys. Rev. Lett. 96 (2006) 014301.  Y. Cheng, J. Xu, X. Liu, Broad forbidden bands in parallel-coupled locally resonant ultrasonic metamaterials, Appl. Phys. Lett. 92 (2008) 051913.  T.-T. Wu, Z.-G. Huang, S. Lin, Surface and bulk acoustic waves in two-dimensional phononic crystal consisting of materials with general anisotropy, Phys. Rev. B 69 (2004) 094301.  H.P. Schriemer, M.L. Cowan, J.H. Page, P. Sheng, Z. Liu, D.A. Weitz, Energy
  
  
velocity of diﬀusing waves in strongly scattering media, Phys. Rev. Lett. 79 (1997) 3166. J.H. Page, P. Sheng, H.P. Schriemer, I. Jones, X. Jing, D.A. Weitz, Group velocity in strongly scattering media, Science (1996) 634–637. S. Benchabane, A. Khelif, J.-Y. Rauch, L. Robert, V. Laude, Evidence for complete surface wave band gap in a piezoelectric phononic crystal, Phys. Rev. E 73 (2006) 065601. S. Mohammadi, A. Adibi, On chip complex signal processing devices using coupled phononic crystal slab resonators and waveguides, AIP Adv. 1 (2011) 041903. J.-N. Gillet, Y. Chalopin, S. Volz, Atomic-scale three-dimensional phononic crystals with a very low thermal conductivity to design crystalline thermoelectric devices, J. Heat Transf. 131 (2009) 043206. P.E. Hopkins, C.M. Reinke, M.F. Su, R.H. Olsson III, E.A. Shaner, Z.C. Leseman, J.R. Serrano, L.M. Phinney, I. El-Kady, Reduction in the thermal conductivity of single crystalline silicon by phononic crystal patterning, Nano Lett. 11 (2010) 107–112. V. Laude, M. Wilm, S. Benchabane, A. Khelif, Full band gap for surface acoustic waves in a piezoelectric phononic crystal, Phys. Rev. E 71 (2005) 036607. M. Travagliati, D. Nardi, C. Giannetti, V. Gusev, P. Pingue, V. Piazza, G. Ferrini, F. Banﬁ, Interface nano-conﬁned acoustic waves in polymeric surface phononic crystals, Appl. Phys. Lett. 106 (2015) 021906. D. Nardi, M. Travagliati, M.M. Murnane, H.C. Kapteyn, G. Ferrini, C. Giannetti, F. Banﬁ, Impulsively excited surface phononic crystals: a route toward novel sensing schemes, IEEE Sens. J. 15 (2015) 5142–5150. S.-Y. Yu, X.-C. Sun, X. Ni, Q. Wang, X.-J. Yan, C. He, X.-P. Liu, L. Feng, M.-H. Lu, Y.F. Chen, Surface phononic graphene, Nat. Mater. 15 (2016) 1243. Z. Liu, X. Zhang, Y. Mao, Y. Zhu, Z. Yang, C.T. Chan, P. Sheng, Locally resonant sonic materials, Science 289 (2000) 1734–1736. R. Sainidou, B. Djafari-Rouhani, Y. Pennec, J. Vasseur, Locally resonant phononic crystals made of hollow spheres or cylinders, Phys. Rev. B 73 (2006) 024302. W. Cheng, J. Wang, U. Jonas, G. Fytas, N. Stefanou, Observation and tuning of hypersonic bandgaps in colloidal crystals, Nat. Mater. 5 (2006) 830–836. D. Leduc, B. Morvan, A. Tinel, R. Sainidou, P. Rembert, Magnetic-sphere-based phononic crystals, Crystals 6 (2016) 78. F. Lucklum, M. Vellekoop, Rapid prototyping of 3D phononic crystals using highresolution stereolithography fabrication, Procedia Eng. 120 (2015) 1095–1098. J.-H. Jang, C.K. Ullal, T. Gorishnyy, V.V. Tsukruk, E.L. Thomas, Mechanically tunable three-dimensional elastomeric network/air structures via interference lithography, Nano Lett. 6 (2006) 740–743. J.-H. Lee, C.Y. Koh, J.P. Singer, S.-J. Jeon, M. Maldovan, O. Stein, E.L. Thomas, 25th anniversary article: ordered polymer structures for the engineering of photons and phonons, Adv. Mater. 26 (2014) 532–569. F. Bloch, Über die quantenmechanik der elektronen in kristallgittern, Z. Phys. A Hadrons Nuclei 52 (1929) 555–600. K. Sakoda, Optical Properties of Photonic Crystals vol. 80, Springer Science & Business Media, 2004. R.C. McMaster, P. Mcintire, M.L. Mester, Nondestructive Testing Handbook: Ultrasonic Testing ASNT, vol. 7, American Society for Nondestructive Testing, Inc, 4153 Arlington Plaza, Columbus, Ohio 43228, USA, 1986, pp. 677. D.L. Bradley, W.D. Wilson, Acoustic Impedance of Sea Water as a Function of Temperature, Pressure and Salinity, Technical Report, Naval Ordnance Laboratory White Oak MD, 1966. J. Lubbers, R. Graaﬀ, A simple and accurate formula for the sound velocity in water, Ultrasound Med. Biol. 24 (1998) 1065–1068. J.H. Page, H.P. Schriemer, I. Jones, P. Sheng, D.A. Weitz, Classical wave propagation in strongly scattering media, Physica A: Stat. Mech. Appl. 241 (1997) 64–71. K. McAuley, The chemistry and physics of polyacrylamide gel dosimeters: why they do and don’t work, Journal of Physics: Conference Series, vol. 3, IOP Publishing, 2004, p. 29. V. Bjerknes, Fields of Force: Supplementary Lectures, Applications to meteorology: A Course of Lectures in Mathematical Physics. December 1 to 23, 1905, 1, The Columbia University Press, 1906.